V2O3/C composite fabricated by carboxylic acid-assisted sol–gel synthesis as anode material for lithium-ion batteries

The potential battery electrode material V2O3/C has been prepared using a sol–gel thermolysis technique, employing vanadyl hydroxide as precursor and different organic acids as both chelating agents and carbon sources. Composition and morphology of resultant materials were characterized by X-ray diffraction, Raman spectroscopy, scanning and transmission electron microscopies, physical sorption, and elemental analysis. Stability and electronic properties of model composites with chemically and physically integrated carbon were studied by means of quantum-chemical calculations. All fabricated composites are hierarchically structured and consist of carbon-covered microparticles assembled of polyhedral V2O3 nanograins with intrusions of amorphous carbon at the grain boundaries. Such V2O3/C phase separation is thermodynamically favored while formation of vanadium (oxy)carbides or heavily doped V2O3 is highly unlikely. When used as anode for lithium-ion batteries, the nanocomposite V2O3/C fabricated with citric acid exhibits superior electrochemical performance with an excellent cycle stability and a specific charge capacity of 335 mAh g−1 in cycle 95 at 100 mA g−1. We also find that the used carbon source has only minor effects on the materials’ electrochemical performance. V2O3/C composites were synthesized by a facile sol–gel thermolysis method. Citric acid, malic acid, and tartaric acid have been applied as both the chelating agents and as carbon source to produce V2O3/C composites for the first time. DFT calculations confirmed preference of phase separation in C-doped V2O3. V2O3/C composites as anode material exhibit an excellent cycle stability. V2O3/C composites were synthesized by a facile sol–gel thermolysis method. Citric acid, malic acid, and tartaric acid have been applied as both the chelating agents and as carbon source to produce V2O3/C composites for the first time. DFT calculations confirmed preference of phase separation in C-doped V2O3. V2O3/C composites as anode material exhibit an excellent cycle stability.


Introduction
Vanadium trioxide V 2 O 3 has been widely studied in fundamental research since the first reports on its metalto-insulator transition [1]. Regarding application, due to its high theoretical capacity (1070 mAh g −1 ), low cost, and non-toxicity V 2 O 3 is well recognized as a promising anode material for rechargeable lithium-ion batteries (LIBs) [2][3][4]. However, the practical use of the bulk V 2 O 3 as anode materials in LIBs is greatly hindered due to huge volume changes appearing upon electrochemical cycling [5]. A variety of functionalization options has been explored to overcome this issues: incorporation of carbon containing compounds yielding composite materials including the preparation of nanosized materials with the different morphology [6,7], doping with nitrogen and sulfur [8][9][10], as well as a design of three-dimensional nanostructures providing shorter lithium-ion/electron diffusion distances as well as more stable structures preventing deterioration of electrodes during the discharge/charge processes [11][12][13][14][15][16].
Both the preparation process and the post-treatment conditions have a significant influence on the electrochemical performances of V 2 O 3 /C hybrid materials as an anode material. For example, V 2 O 3 /C composites prepared by a NaCl template-assisted freeze-drying strategy deliver a capacity of 706 mAh g −1 at 5 A g −1 , after 2000 cycles [17], while electrospun materials show 100 mAh g −1 at 5000 A g −1 after 5000 cycles [18]. Among different kinds of carbon materials, there is a variety of reports using graphene oxide (rGO) as the carbon source [5,19,20], among them a polymer-pyrolysis made material with~780 mAh g −1 over 100 cycles at 200 mA g −1 [21] and V 2 O 3 /rGO with 823 mAh g −1 , at 0.1 A g −1 [22]. Other V 2 O 3 /C composites have been fabricated by solvothermal synthesis using ethylene glycol as the carbon source (474 mAh g −1 at 0.5 A g −1 after 400 cycles) [23], a hydrothermal route and subsequent calcinations (283 mAh g −1 at 25 A g −1 ) [24].
Here we report for the first time a sol-gel process with post-annealing treatment to synthesize a V 2 O 3 /C composite material using citric acid, tartaric acid, and malic acid as both the chelating agents and the carbon sources. In general, the sol-gel method has been extensively used to synthesize electrode materials due to their unique advantages such as low synthesis temperature, high purity and high homogeneous structure, and good electrochemical property of the synthesized product [25][26][27][28]. Our work shows that it can be exploited as facile method to synthesize hierarchically structured V 2 O 3 /C nanocomposite and we investigate in detail the influence of different carboxylic acids on the phase composition, morphology, and electrochemical properties of the products. 2.2 Synthesis of V 2 O 3 /C composites V 2 O 3 /C composites were prepared using the sol-gel thermolysis process. The typical synthesis process is briefly described as follows. First, vanadyl hydroxide VO(OH) 2 precursor was prepared. According to the synthetic procedure, 7.95 g VOSO 4 ·nH 2 O was dissolved in 400 mL of deionized H 2 O using the magnetic stirring at room temperature, then ammonium hydroxide solution was added dropwise to adjust the pH value of the mixture so that it equals to 4. The brown precipitate was collected by centrifugation and washed several times with water, ethanol, and dried in air to obtain the VO(OH) 2 powder products. Second, VO(OH) 2 and carboxylic acid (citric acid, malic acid or tartaric acid) were weighed according to the molar ration of 1:1 and mixed well with each other in deionized 60 mL water under constantly stirring. The mixture then came to be a blue solution. The blue solution was evaporated at 80°C for~4 h, with a magnetic stirrer sequentially stirring to obtain a clear viscous sol and was subsequently dried to form a gel. The gel was further dried in a vacuum oven at 50°C for 16 h, which led to a blue powder. Finally, the powder was sintered under a flow of N 2 gas at 400-700°C for 1 h to obtain the V 2 O 3 /C composites. Depending on the type of the carboxylic acids, the resulting materials are denoted henceforth as V 2 O 3 /C-C, V 2 O 3 /C-M, and V 2 O 3 /C-T, where carboxylic acid is citric acid, malic acid, and tartaric acid, respectively.

Characterization
X-ray diffraction (XRD) patterns were obtained using a Bruker AXS D8 Advance Eco diffractometer using CuKα radiation and applying the step size of Δ2θ = 0.02°. The morphology of the powder was determined by a ZEISS Leo 1530 scanning electron microscope (SEM) as well as JEOL JEM 2100 and JEMe200 CX high-resolution transmission electron microscopes (HRTEM). The thermogravimetric analysis with the heating rate of 10 K min −1 under flowing air was carried out using a STA 449 F 3 Jupiter thermoanalyzer (Netzsch) coupled with a QMS 403 mass spectrometer (TG-DSC-MS). The specific surface area and pore volume of the samples were measured by a surface area and porosity analyzer (Gemine VII, Micromeritics). The content of carbon was examined by elemental chemical analysis (CA) using Vario MICRO Cubes (Elementar). Prior to N 2 physisorption data collection, the samples were degassed at 100°C under vacuum for 1.5 h. The specific surface area, pore size distribution, and pore volumes were obtained by means of the Brunauer-Emmett-Teller (BET) method and the Barrett-Joyner-Halenda model from the adsorption branches of the isotherms. Raman spectra were measured with a Renishaw U1000 spectroscope at a laser wavelength of 532 nm.

Computational details
All quantum-chemical calculations of the V 2 O 3 /C composite systems were performed within the framework of the selfconsistent-charge density-functional tight-binding method (SCC-DFTB) [29,30]. Atomic positions in both the supercells of the bulk V 2 O 3 doped by carbon and the supercells of a slab V 2 O 3 (0001) contacting with graphene were optimized using the conjugate gradient algorithm within periodic boundary conditions in Г-point approximation. Self-consistent calculations were performed until the maximal residual components for the total energy of 10 −3 eV atom −1 and for the interatomic force component of 10 −2 eV Å −1 . The lattice parameters optimized within these conditions for the bulk V 2 O 3 are in a fair agreement with the experimental values, being overestimated by 3% (a = 5.07 Å, c = 14.25 Å).
As the progenitor of all the model V 2 O 3 /C composites the pre-optimized supercell 2a × 2a × 1c of bulk V 2 O 3 was selected. Several possible variants for distribution of carbon impurities within V 2 O 3 lattice have been accounted: substitutional single C atoms within V or O sublattices; substitutional C 2 dimers at neighbor sites within V or/and O sublattices; interstitial single C atoms or C 2 dimers; graphene sheet on a V 2 O 3 surface. The relative stability of these V 2 O 3 /C composites with relaxed internal geometry was analyzed using the energy of formation ΔE relative to corresponding mechanistic mixture of the bulk V 2 O 3 , graphite and molecular CO. Positive and negative ΔE values point to endo-and exothermic formation reaction, respectively.

Electrochemical measurements
The electrochemical measurements of the samples were performed with a VMP3 potentiostat (Bio-Logic SAS) at 25°C using Swagelok-type half cells with lithium metal foil (Alfa Aesar) as counter electrode [31]. The electrodes were separated by two layers of glass fiber separator (Whatman GF/D) that was soaked with 200 μL of a 1 M LiPF 6 salt solution in 1:1 ethylene carbonate and dimethyl carbonate (Merck Electrolyte LP30). The working electrode consists of active material, carbon black (Super C65, Timcal) and polyvinylidene fluoride binder (Solvay Plastics) in a weight ratio of 75:15:10. The powders were mixed in N-methyl-2pyrrolidone (NMP, Sigma-Aldrich) and stirred for at least 12 h. After evaporating most of the NMP under vacuum the spreadable slurry was deposited on circular Cu meshes (diameter 10 mm) with a mass loading of about 0.4-0.5 mg cm −2 . Afterward, the electrodes were dried under vacuum, pressed with a spindle press by hand and then dried again. The preparation of the electrodes and the cell assembly were done in a glovebox filled with argon (O 2 /H 2 O < 5 ppm). The calculation of the specific capacity is based on the total mass weight of the composites V 2 O 3 /C.

Results and discussion
XRD patterns of the V 2 O 3 /C composites prepared using different carboxylic acids at different temperatures are depicted in Fig. 1a. All samples obtained after annealing at temperatures below 700°C are amorphous according to the XRD patterns as demonstrated by the example of the V 2 O 3 / C-C composite. Annealing at 700°C leads to the appearance of distinguished XRD patterns, which can be undoubtedly attributed to V 2 O 3 without any impurities. The lattice of V 2 O 3 within the as-prepared V 2 O 3 /C composites has rhombohedral crystalline structure and belongs to the R-3c space group. For all crystalline V 2 O 3 /C materials reported here, the lattice parameters derived from the XRD data are listed in Table 1. The results are found close to the reported values for V 2 O 3 [ICSD No. 94768]. The XRD patterns however display rather broad and low-intense diffraction peaks, which may be attributed to both a poor crystallinity or/and to a small crystal size of primary V 2 O 3 particles present in the composites. Using Scherrer's equation enables estimating the average crystallite sizes of V 2 O 3 particles: where D hkl is the extent of the crystal perpendicular to the reflecting hkl-crystal plane, K is a constant depending on the crystal shape which can be approximated to 0.9, λ is the wavelength of the applied CuKα radiation, Δ(2θ hkl ) is the full width at half-maximum of the diffraction peak, and θ hkl is the Bragg angle. The average crystallite sizes of V 2 O 3 particles obtained from the analysis of the (012), (104), (110), and (116) reflexes are presented in Table 1. All materials exhibit nanosized primary particles with similar size. Obviously, the crystallite size does not seem to be affected by the chelating agent, which was also observed for other oxide systems, for example, Y 3 Fe 5 O 12 and Y 2 O 3 synthesized by sol-gel technique with citric, malic, or tartaric acid [32,33]. This phenomenon is attributed to the space steric effect of the organic acids playing the role of the chelating agent [34]. The chelating ability of carboxylic acids depends on the presence of the carboxylic -COOH groups. Citric acid in comparison with both malic acid and tartaric acid has three -COOH groups, which promote the formation of vanadium-ligand bonds, the formation of a chelate complex, and the growth of crystallites. However, the intermolecular steric hindrances are formed between the citric acid molecules and metal oxide due to the large molecular weight of the citric acid. A large space steric effect hinders close contact between the chelating agent and vanadium oxide that does not favor the growth of V 2 O 3 particles. The main difference in the XRD patterns of the three composites is the relative intensity of the V 2 O 3 reflexes. For the composite prepared using malic acid the ratio of the area of all crystalline peaks to the total area of the diffractogram is slightly higher than those for V 2 O 3 /C-C and V 2 O 3 /C-T indicating higher crystallinity of V 2 O 3 . This shows that malic acid is an eminent chelating agent to synthesize V 2 O 3 /C composite with higher crystallinity. Similar results were also observed in the synthesis of LiV 3 O 8 prepared by sol-gel method and post-annealing treatment with citric, malic, and tartaric acid as chelating agents [35]. Raman spectroscopy provides further information about the structure of V 2 O 5 and also on the carbon in the V 2 O 3 /C composites. All peaks shown in Fig. 1b located below 1000 cm −1 can be attributed to V-O vibrations of V 2 O 5 in agreement with the literature values [36]. Evidently, V 2 O 3 is partially oxidized to V 2 O 5 under the laser irradiation during the Raman measurement in air [37] and therefore, the spectra also show characteristic Raman modes of the V 2 O 5 phase. In addition, two broad peaks at~1350 cm −1 and~1600 cm −1 are clearly observed in the spectra of V 2 O 3 /C composites (Fig. 1c). The band at~1600 cm −1 labeled as the G-band is related to the in-plane vibration of sp 2 hybridized carbon atoms [38][39][40], while the one at about 1350 cm −1 labeled as the D-band is associated to the breathing mode of sp 2 atoms in rings and only becomes active in the presence of defects [38][39][40]. The peaks of D-and G-bands are broad implying that carbon possesses high structural disorder [39,41,42]. The ratio of the  In comparison with citric acid and malic acid as the chelating agent, this ratio is for V 2 O 3 /C-T composite slightly higher indicating less defects and disorder in the carbon component [38]. Thermogravimetric analyses coupled with massspectroscopy confirm the presence of carbon and allow to derive the carbon content in the V 2 O 3 /C composites under study (Fig. 2). The TG-DSC-MS curves of the composites prepared by citric acid (Fig. 2a), malic acid (Fig. 2b), and tartaric acid (Fig. 2c) are very similar. For all three composites, the weight loss proceeds stepwise. In the first step ranged from room temperature to about 180°C, there is a weak endothermic peak signaling the vaporization of adsorption water. The corresponding weight loss is about 3.1−4.8 wt%. A second step ranging from 200 to 560°C implies two strong exothermic peaks, which are associated with the vigorous combustion reactions of the carbon component in the composites and the completion of the crystallization reaction. The release of carbon dioxide CO 2 is confirmed by two intense peaks from molecular ion CO 2 + with m/z = 44 a.m.u. in the mass spectra. Seemingly, the existence of this double exotherm with well-resolvable temperature maxima is due to the different states of carbon in the composites. A last feature is observed from~500 to 730°C. Here, there is a weight gain of 1.6, 1.  Table 1). The morphologies of the V 2 O 3 /C powders synthesized from citric acid, malic acid, and tartaric acid as carbon source are similar. All of them show micrometer sized chunks (Fig. S1) that are decorated with flake-like particles with the average flake size of 100-300 nm and 30-40 nm in thickness (Fig. 3a-c). In addition, the detailed microstructure of the V 2 O 3 /C-C composite studied by TEM (Fig. 3d) displays a block-like architecture of particles on the nanometer scale. The TEM images also show an amorphous carbon layer of up to 100 nm in thickness. Nanoparticles with the shape of edge-shared polyhedra are uniformly and tightly anchored to an amorphous carbon matrix (Fig. 3e). The lattice fringes with spacing of 0.37 nm corresponds to the (012) plane of the rhombohedral V 2 O 3 phase. The corresponding ring-like selected-area electron diffraction (SAED) pattern (Fig. 3f) indicates that the as-synthesized composite is a polycrystalline phase indexed to V 2 O 3 , which is consistent with the XRD results presented above. Textural properties of the differently prepared V 2 O 3 /C composites as obtained from nitrogen adsorption and desorption studies and their analysis are shown in Fig. S2 and in Table 1. According to the IUPAC classification, the nitrogen adsorption/desorption isotherms display a type IV behavior [43].
In summary, analysis of XRD, SEM, TEM, and BET data provides solid evidence that the materials exhibit tightly bound, yet, separated V 2 O 3 and carbon phases. However, doping of carbon into the V 2 O 3 lattice cannot be completely excluded, since it remains undetectable by these methods. Therefore, quantum-chemical DFTB calculations have been employed to estimate tendency of the V 2 O 3 lattice to host substitutional and/ or interstitial carbon impurities. Several model variants of single and paired carbon atoms hosted at O-or V sites or as  (Table S1). An essential difference in their relative thermodynamic stabilities is established after comparison of their formation energies ΔE. There are a few important inferences. Namely, substitution of single O atoms by C atoms within V 2 O 3 , accompanied by emergence of carbide-like V-C bonding, is endothermic. Moreover, clusterization of such C atoms is even less favorite. Implantation of interstitial C atoms is also characterized by endothermic energies irrespective of the carbons' mutual distribution.
The energetically most beneficial and even exothermic carbon distribution has been found for the variants of cooperative substitution of either two neighboring V atoms or an VO unit (see Table S1). Optimized structures including these defects undergo a considerable evolution, compared to their initial geometries, which is accompanied by a contraction in the neighborhood of the defect, i.e., by the appearance of a nanoscopic cavity within the bulk of V 2 O 3 . Particularly, substitution of neighboring V and O atoms leads to the formation of acetylide-like dimers bound via an atom to two V atoms (Table S1, defect type 8). Though, the energetically most beneficial cooperative substitution is found to be on two neighboring V sites, which results in the formation of CO molecules within nanoscopic cavity. Depending on the initial positions of substituting C atoms, the final structure contains either two CO molecules (Table  S1, defect type 10) or a single CO molecule and a carbonatelike group (Table S1, defect type 11, and Fig. S3).
Beside the formation of molecular-like carbon species or carbon oxides, the release of free carbon in bulk quantities like a graphene sheet on the V 2 O 3 (0001) surface should be also an exothermic reaction (Table S1, defect type 14, and Fig. S3). Noteworthy, the in-plane lattice parameters of a V 2 O 3 (0001) surface and graphene commensurate very well with a ratio close to a V2O3 ≈ 2a C . According to our calculations, the only stable type of V 2 O 3 (0001) surface appears as stoichiometric surface with the V atoms moved inward to the surface layer. The graphene sheet can stay 3.1 Å away from this reconstructed surface.
Despite the exclusively thermodynamic characterization, the calculations are capable to explain the origin of several morphological features established in the experimentally fabricated V 2 O 3 /C composites. Irrespective of the mechanism for reduction of V 5+ from metal-organic precursors, the formation of any vanadium carbides, vanadium oxycarbides or stable (V,C) 2 O 3 solid solutions within the V 2 O 3 /C system should be not expected. Any possible (V,C) 2 O 3 intermediate should decompose into a thermodynamically more stable state, namely, the nanocavernous bulk V 2 O 3 with CO or C 2 species residing in the caverns. Such structural faults do not promote the mechanical stability of the lattice and can serve as the origins of cracks with degassing of fugitive components. The higher the content of the faults, the smaller domains of forming V 2 O 3 should be observed. After all, the most likely forms of carbon in the V 2 O 3 /C In addition, the calculations give a preliminary estimate of the electronic structure of V 2 O 3 /C composites. The electronic densities-of-states (DOS) are typical for the metal-like compounds, and the origin of the DOS near the Fermi level remains similar irrespective of the carbon type in a composite. It is contributed mostly from the V3dstates of the V 2 O 3 part. The examples for the most thermodynamically stable V 2 O 3 /C composites-with either chemically integrated or elemental carbon-are depicted in Fig. 4. Similarly to the pristine V 2 O 3 , the Fermi level is hosted in a local DOS minimum of the wide V3d-band, hence, all composites should have a metal-like conductivity. Valence O2p states form the wide band at −8…−4 eV below the Fermi level. Chemically integrated carbon (like molecular-like СО or C 2 ) donates also occupied С2p states to both the top and the bottom of the main valence band (Fig. 4а). In the case of physisorbed carbon like graphene in contact to the V 2 O 3 (0001) surface, the valence С2p states demonstrate an essential dispersion, though, they are missing at the Fermi level (Fig. 4b). Here, V3d states near the Fermi level are presented by both the bulk and the surface V atoms. Thus, all V 2 O 3 /C composites should preserve a metal-like type of conductivity like parent V 2 O 3 .
Electrochemical properties of the V 2 O 3 /C composites synthesized with different carbon sources are investigated by cyclic voltammetry (CV) and galvanostatic cycling with potential limitation (GCPL) in the voltage range between 0.01 V and 3.2 V. Exemplary for all samples, Fig. 5a shows the first, second, and fifth cycle of the cyclic voltammogram of V 2 O 3 /C-M recorded at a scan rate of 0.05 mV s −1 . As shown in Fig. S4, the CV curves of the other two composites, V 2 O 3 /C-C and V 2 O 3 /C-T, exhibit the same features.
Starting with a reductive scan in the first cycle a peak R SEI at around 0.75 V occurs mainly due to the irreversible formation of a solid electrolyte interface (SEI) [21]. The redox peak pair R C /O C around the lower limit 0.01 V corresponds to the lithiation and delithiation of the carbon [44]. All other features, the reduction peaks R 1 and R 2 as well as the oxidation peaks O1 and O2, can be assigned to the electrochemical reactions of V 2 O 3 . The Li + storage of V 2 O 3 initially runs via intercalation (Eq. 2) and, subsequently, conversion of Li x V 2 O 3 to metallic V and Li 2 O (Eq. 3) as follows [2,45]: In the CV curve, there are two broad reduction peaks at 0.9 and 1.75 V and two oxidation peaks at 1.25 and 2.5 V. The absence of much more pronounced peaks implies that the de-/lithiation process smoothly proceeds with several transition species originating from the multivalence of vanadium [21,46]. The cycling performances of the different samples are studied by GCPL measurements. In Fig. 5b, the dis-/charge capacities at 100 mA g −1 are shown. The first dis-/charge capacities of V 2 O 3 /C-C, V 2 O 3 /C-M, and V 2 O 3 /C-T are 769/ 302, 763/358, and 612/257 mAh g −1 , respectively. The huge discrepancy between the first discharge and charge capacity is caused by the irreversible SEI formation and structural changes during the first lithiation [2,7,24]. Upon further cycling, the capacity initially rises slightly, which can be attributed to an activation process as a result of electrochemical grinding. This phenomenon has been observed in literature for V 2 O 3 -based electrodes [7,21] as well as other anode materials [47,48]. During the whole measurement the samples exhibit a high cycle stability, whereas especially V 2 O 3 /C-C stands out. It convinces with a capacity retention of 98% in cycle 95 relative to cycle 33, where the maximal charge capacity of 342 mAh g −1 is obtained. By comparing the composites among each other no clear differences of the electrochemical performance can be observed. As expected, due to the quite similar physical properties of the different composites, the used carbon source (citric acid, malic acid or tartaric acid) does not strongly affect the electrochemical properties. In Fig. 5c, the specific dis-/charge capacities are shown at different current rates between 100 and 500 mA g −1 . The composite V 2 O 3 /C-M is superior and exhibits specific charge capacities of 337, 269, and 183 mAh g −1 at current densities of 100, 200, and 500 mA g −1 after 15 cycles each. When the current density is returned to 100 mA g −1 a charge capacity of 327 mAh g −1 is regained, demonstrating excellent capacity retention. The other two samples also exhibit high rate performance. The dis-/charge profiles (Fig. S5b) reveal no significant differences of the overpotential due to polarization effects for the different composites. The slightly better rate capacity of V 2 O 3 /C-M compared to V 2 O 3 /C-T may be due to an improved electronic conductivity of the material. The percolation threshold for forming a conductive network in a randomly packed threedimensional body consisting of conductive and insulating particles is exceeded by the higher carbon content, which ensures higher conductivity in the V 2 O 3 /C-M composite, and thus achieves superior performance [49,50]. The fact that the composite V 2 O 3 /C-C with the highest carbon content shows lower rate capacity as V 2 O 3 /C-M might be due the less amount of the active material, V 2 O 3 , in the anode material that comes along with it [49].
For a comparison, the electrochemical performances of V 2 O 3 /C composites prepared via different synthesis methods are collected in Table 2. It can be concluded that the composites presented in this work lie in the midfield. The outstanding performance of V 2 O 3 /C nanocomposites prepared through the thermolysis of a polymer matrix-based metal precursor can possibly be explained by the good distribution of both components.

Conclusions
In summary, we demonstrate a facile, low cost, and scalable two-step route to fabricate pure vanadium-based V 2 O 3 /C composites of polynanocrystalline V 2 O 3 microparticles encapsulated in an amorphous carbon matrix. The absence of foreign phases is confirmed by means of several physical and analytical methods, while the existence of the few-atom impurities has been criticized using quantum-chemical calculations. Based on theoretical analysis, the formation mechanism of such structured composites might include formation of molecular CO, carbonate ions and progressive growth of C-C chains all upon carbonization of precursors. Diffusion out of decomposing precursor and outgassing of these species leads to extensive fracturing of emerging V 2 O 3 lattice and to the elemental carbon remained at surface of V 2 O 3 .
A slight regulation of the carbon content, the typical size of V 2 O 3 nanocrystallites and, consequently, the accessible physical surface of the product can be attained using different precursors-vanadyl complexes with citric, tartaric, or malic acids. However, electrochemical performance of the final products as anode materials for LIBs are not strongly affected by the type of carbon source. Slight differences in the rate capacity may be due to different carbon contents. All our V 2 O 3 /C composites exhibit an excellent cycle stability at a medium-range reversible capacity in-line with formerly known V 2 O 3 /C composites.

Compliance with ethical standards
Conflict of interest The authors declare no competing interests.
Publisher's note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article's Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article's Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons. org/licenses/by/4.0/.